data_LI03_ND_CIF_publ

_pd_block_id
  2014-07-31T14:58|LI03_ND_CIF|Young-Il_Kim|Overall

_audit_creation_method  "from EXP file using GSAS2CIF"
_audit_creation_date                   2014-07-31T14:58
_audit_author_name                     "Young-Il Kim"
_audit_update_record
; 2014-07-31T14:58  Initial CIF as created by GSAS2CIF
;

#=============================================================================
# this information describes the project, paper etc. for the CIF             #
# Acta Cryst. Section C papers and editorial correspondence is generated     #
# from the information in this section                                       #
#                                                                            #
#   (from)   CIF submission form for Rietveld refinements (Acta Cryst. C)    #
#                                                 Version 14 December 1998   #
#=============================================================================
# 1. SUBMISSION DETAILS

_publ_contact_author_name            ?   # Name of author for correspondence
_publ_contact_author_address             # Address of author for correspondence
; ?
;
_publ_contact_author_email           ?
_publ_contact_author_fax             ?
_publ_contact_author_phone           ?

_publ_contact_letter
; ?
;

_publ_requested_journal              ?
_publ_requested_coeditor_name        ?
_publ_requested_category             ?   # Acta C: one of CI/CM/CO/FI/FM/FO

#==============================================================================

# 2. PROCESSING SUMMARY (IUCr Office Use Only)

_journal_data_validation_number      ?

_journal_date_recd_electronic        ?
_journal_date_to_coeditor            ?
_journal_date_from_coeditor          ?
_journal_date_accepted               ?
_journal_date_printers_first         ?
_journal_date_printers_final         ?
_journal_date_proofs_out             ?
_journal_date_proofs_in              ?
_journal_coeditor_name               ?
_journal_coeditor_code               ?
_journal_coeditor_notes
; ?
;
_journal_techeditor_code             ?
_journal_techeditor_notes
; ?
;
_journal_coden_ASTM                  ?
_journal_name_full                   ?
_journal_year                        ?
_journal_volume                      ?
_journal_issue                       ?
_journal_page_first                  ?
_journal_page_last                   ?
_journal_paper_category              ?
_journal_suppl_publ_number           ?
_journal_suppl_publ_pages            ?

#==============================================================================

# 3. TITLE AND AUTHOR LIST

_publ_section_title
; ?
;
_publ_section_title_footnote
; ?
;

# The loop structure below should contain the names and addresses of all
# authors, in the required order of publication. Repeat as necessary.

loop_
	_publ_author_name
        _publ_author_footnote
	_publ_author_address
 ?                                   #<--'Last name, first name'
; ?
;
; ?
;

#==============================================================================

# 4. TEXT

_publ_section_synopsis
;  ?
;
_publ_section_abstract
; ?
;
_publ_section_comment
; ?
;
_publ_section_exptl_prep      # Details of the preparation of the sample(s)
                              # should be given here.
; ?
;
_publ_section_exptl_refinement
; ?
;
_publ_section_references
; ?
;
_publ_section_figure_captions
; ?
;
_publ_section_acknowledgements
; ?
;

#=============================================================================
# 5. OVERALL REFINEMENT & COMPUTING DETAILS

_refine_special_details
; ?
;
_pd_proc_ls_special_details
; ?
;

# The following items are used to identify the programs used.
_computing_molecular_graphics     ?
_computing_publication_material   ?

_refine_ls_weighting_scheme       ?
_refine_ls_weighting_details      ?
_refine_ls_hydrogen_treatment     ?
_refine_ls_extinction_method      ?
_refine_ls_extinction_coef        ?
_refine_ls_number_constraints     ?

_refine_ls_restrained_S_all       ?
_refine_ls_restrained_S_obs       ?

#==============================================================================
# 6. SAMPLE PREPARATION DATA

# (In the unusual case where multiple samples are used in a single
#  Rietveld study, this information should be moved into the phase
#  blocks)

# The following three fields describe the preparation of the material.
# The cooling rate is in K/min.  The pressure at which the sample was
# prepared is in kPa.  The temperature of preparation is in K.

_pd_prep_cool_rate                ?
_pd_prep_pressure                 ?
_pd_prep_temperature              ?

_pd_char_colour                   ?       # use ICDD colour descriptions
data_LI03_ND_CIF_overall

_refine_ls_shift/su_max                15.37
_refine_ls_shift/su_mean               0.55
_computing_structure_refinement        GSAS
_refine_ls_number_parameters           29
_refine_ls_goodness_of_fit_all         2.77
_refine_ls_number_restraints           0
_refine_ls_matrix_type                 full

# pointers to the phase blocks
loop_   _pd_phase_block_id
      2014-07-31T14:58|LI03_ND_CIF_phase1|Young-Il_Kim||
# pointers to the diffraction patterns
loop_   _pd_block_diffractogram_id
      ?

# Information for phase 1
data_LI03_ND_CIF_phase_1

_pd_block_id
  2014-07-31T14:58|LI03_ND_CIF_phase1|Young-Il_Kim||

#==============================================================================
# 7. CHEMICAL, STRUCTURAL AND CRYSTAL DATA

_pd_char_particle_morphology      ?

_chemical_name_systematic
; ?
;
_chemical_name_common             ?
_chemical_formula_moiety          ?
_chemical_formula_structural      ?
_chemical_formula_analytical      ?
_chemical_melting_point           ?
_chemical_compound_source         ?       # for minerals and
                                          # natural products
_symmetry_space_group_name_Hall   ?

_exptl_crystal_F_000               ?
_exptl_crystal_density_diffrn      ?
_exptl_crystal_density_meas        ?
_exptl_crystal_density_method      ?

_cell_measurement_temperature     ?

_cell_special_details
; ?
;

_geom_special_details             ?

# The following item identifies the program(s) used (if appropriate).
_computing_structure_solution     ?

#==============================================================================

# 8. Phase information from GSAS

_pd_phase_name                         I4/mcm
_cell_length_a                         5.69071(15)
_cell_length_b                         5.69071
_cell_length_c                         8.0673(5)
_cell_angle_alpha                      90.0
_cell_angle_beta                       90.0
_cell_angle_gamma                      90.0
_cell_volume                           261.253(15)
_symmetry_cell_setting                 tetragonal
_symmetry_space_group_name_H-M         "I 4/m c m"
loop_ _symmetry_equiv_pos_site_id _symmetry_equiv_pos_as_xyz
       1 +x,+y,+z 
       2 -y,+x,+z 
       3 -x,-y,+z 
       4 +y,-x,+z 
       5 -x,+y,+z+1/2 
       6 -y,-x,+z+1/2 
       7 +x,-y,+z+1/2 
       8 +y,+x,+z+1/2 
      -1 -x,-y,-z 
      -2 +y,-x,-z 
      -3 +x,+y,-z 
      -4 -y,+x,-z 
      -5 +x,-y,-z+1/2 
      -6 +y,+x,-z+1/2 
      -7 -x,+y,-z+1/2 
      -8 -y,-x,-z+1/2 
     101 +x+1/2,+y+1/2,+z+1/2 
     102 -y+1/2,+x+1/2,+z+1/2 
     103 -x+1/2,-y+1/2,+z+1/2 
     104 +y+1/2,-x+1/2,+z+1/2 
     105 -x+1/2,+y+1/2,+z 
     106 -y+1/2,-x+1/2,+z 
     107 +x+1/2,-y+1/2,+z 
     108 +y+1/2,+x+1/2,+z 
    -101 -x+1/2,-y+1/2,-z+1/2 
    -102 +y+1/2,-x+1/2,-z+1/2 
    -103 +x+1/2,+y+1/2,-z+1/2 
    -104 -y+1/2,+x+1/2,-z+1/2 
    -105 +x+1/2,-y+1/2,-z 
    -106 +y+1/2,+x+1/2,-z 
    -107 -x+1/2,+y+1/2,-z 
    -108 -y+1/2,-x+1/2,-z 

# ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS


loop_
      _atom_site_type_symbol
      _atom_site_label
      _atom_site_fract_x
      _atom_site_fract_y
      _atom_site_fract_z
      _atom_site_occupancy
      _atom_site_thermal_displace_type
      _atom_site_U_iso_or_equiv
      _atom_site_symmetry_multiplicity
Sr
Sr      0.0          0.5          0.25         0.73       Uiso   0.0070(4)     4
Ta
Ta      0.0          0.0          0.0          0.73       Uiso   0.0008(4)     4
Li
Li      0.0          0.0          0.0          0.27       Uiso   0.0008(4)     4
O 
O1      0.0          0.0          0.25         0.169(17)  Uiso   0.0223(4)     4
N 
N1      0.0          0.0          0.25         0.331(17)  Uiso   0.0223(4)     4
O 
O2      0.77262(20)  0.27262(20)  0.0          0.825(8)   Uiso   0.0223(4)     8
N 
N2      0.77262(20)  0.27262(20)  0.0          0.125(8)   Uiso   0.0223(4)     8

loop_ _atom_type_symbol
      _atom_type_number_in_cell
                   Sr  2.92       
                   Ta  2.92       
                   Li  1.08       
                   O   7.28       
                   N   2.32       
 
# If you change Z, be sure to change all 3 of the following
_chemical_formula_sum                  "Li1.08 N2.32 O7.28 Sr2.92 Ta2.92"
_chemical_formula_weight               940.68
_cell_formula_units_Z                  1

# MOLECULAR GEOMETRY

loop_
      _geom_bond_atom_site_label_1
      _geom_bond_atom_site_label_2
      _geom_bond_distance
      _geom_bond_site_symmetry_1
      _geom_bond_site_symmetry_2
      _geom_bond_publ_flag
  Sr        Sr             4.02394(11)  .      2_555  N
  Sr        Sr             4.02394(11)  .      2_565  N
  Sr        Sr             4.02394(11)  .      2_655  N
  Sr        Sr             4.02394(11)  .      2_665  N
  Sr        Sr             4.03365(23)  .      5_554  N
  Sr        Sr             4.03365(23)  .      5_555  N
  Sr        Ta              3.48764(9)  .      1_555  N
  Sr        Ta              3.48764(9)  .      1_565  N
  Sr        Ta              3.48764(9)  .      5_555  N
  Sr        Ta              3.48764(9)  .      5_565  N
  Sr        Ta              3.48764(9)  .    101_455  N
  Sr        Ta              3.48764(9)  .    101_555  N
  Sr        Ta              3.48764(9)  .    105_455  N
  Sr        Ta              3.48764(9)  .    105_555  N
  Sr        Li              3.48764(9)  .      1_555  N
  Sr        Li              3.48764(9)  .      1_565  N
  Sr        Li              3.48764(9)  .      5_555  N
  Sr        Li              3.48764(9)  .      5_565  N
  Sr        Li              3.48764(9)  .    101_455  N
  Sr        Li              3.48764(9)  .    101_555  N
  Sr        Li              3.48764(9)  .    105_455  N
  Sr        Li              3.48764(9)  .    105_555  N
  Sr        O1              2.84535(8)  .      1_555  N
  Sr        O1              2.84535(8)  .      1_565  N
  Sr        O1              2.84535(8)  .    105_455  N
  Sr        O1              2.84535(8)  .    105_555  N
  Sr        N1              2.84535(8)  .      1_555  N
  Sr        N1              2.84535(8)  .      1_565  N
  Sr        N1              2.84535(8)  .    105_455  N
  Sr        N1              2.84535(8)  .    105_555  N
  Sr        O2              2.7233(11)  .      1_455  N
  Sr        O2              2.9801(12)  .      2_555  N
  Sr        O2              2.7233(11)  .      3_665  N
  Sr        O2              2.9801(12)  .      4_565  N
  Sr        O2              2.7233(11)  .      5_655  N
  Sr        O2              2.9801(12)  .      6_565  N
  Sr        O2              2.7233(11)  .      7_465  N
  Sr        O2              2.9801(12)  .      8_555  N
  Sr        N2              2.7233(11)  .      1_455  N
  Sr        N2              2.9801(12)  .      2_555  N
  Sr        N2              2.7233(11)  .      3_665  N
  Sr        N2              2.9801(12)  .      4_565  N
  Sr        N2              2.7233(11)  .      5_655  N
  Sr        N2              2.9801(12)  .      6_565  N
  Sr        N2              2.7233(11)  .      7_465  N
  Sr        N2              2.9801(12)  .      8_555  N
  Ta        Sr              3.48764(9)  .      1_545  N
  Ta        Sr              3.48764(9)  .      1_555  N
  Ta        Sr              3.48764(9)  .      2_555  N
  Ta        Sr              3.48764(9)  .      2_655  N
  Ta        Sr              3.48764(9)  .      5_544  N
  Ta        Sr              3.48764(9)  .      5_554  N
  Ta        Sr              3.48764(9)  .      6_554  N
  Ta        Sr              3.48764(9)  .      6_654  N
  Ta        O1             2.01683(11)  .      1_555  N
  Ta        O1             2.01683(11)  .      5_554  N
  Ta        N1             2.01683(11)  .      1_555  N
  Ta        N1             2.01683(11)  .      5_554  N
  Ta        O2             2.02018(16)  .      1_455  N
  Ta        O2             2.02018(16)  .      2_545  N
  Ta        O2             2.02018(16)  .      3_655  N
  Ta        O2             2.02018(16)  .      4_565  N
  Ta        N2             2.02018(16)  .      1_455  N
  Ta        N2             2.02018(16)  .      2_545  N
  Ta        N2             2.02018(16)  .      3_655  N
  Ta        N2             2.02018(16)  .      4_565  N
  Li        Sr              3.48764(9)  .      1_545  N
  Li        Sr              3.48764(9)  .      1_555  N
  Li        Sr              3.48764(9)  .      2_555  N
  Li        Sr              3.48764(9)  .      2_655  N
  Li        Sr              3.48764(9)  .      5_544  N
  Li        Sr              3.48764(9)  .      5_554  N
  Li        Sr              3.48764(9)  .      6_554  N
  Li        Sr              3.48764(9)  .      6_654  N
  Li        O1             2.01683(11)  .      1_555  N
  Li        O1             2.01683(11)  .      5_554  N
  Li        N1             2.01683(11)  .      1_555  N
  Li        N1             2.01683(11)  .      5_554  N
  Li        O2             2.02018(16)  .      1_455  N
  Li        O2             2.02018(16)  .      2_545  N
  Li        O2             2.02018(16)  .      3_655  N
  Li        O2             2.02018(16)  .      4_565  N
  Li        N2             2.02018(16)  .      1_455  N
  Li        N2             2.02018(16)  .      2_545  N
  Li        N2             2.02018(16)  .      3_655  N
  Li        N2             2.02018(16)  .      4_565  N
  O1        Sr              2.84535(8)  .      1_545  N
  O1        Sr              2.84535(8)  .      1_555  N
  O1        Sr              2.84535(8)  .      2_555  N
  O1        Sr              2.84535(8)  .      2_655  N
  O1        Ta             2.01683(11)  .      1_555  N
  O1        Ta             2.01683(11)  .      5_555  N
  O1        Li             2.01683(11)  .      1_555  N
  O1        Li             2.01683(11)  .      5_555  N
  N1        Sr              2.84535(8)  .      1_545  N
  N1        Sr              2.84535(8)  .      1_555  N
  N1        Sr              2.84535(8)  .      2_555  N
  N1        Sr              2.84535(8)  .      2_655  N
  N1        Ta             2.01683(11)  .      1_555  N
  N1        Ta             2.01683(11)  .      5_555  N
  N1        Li             2.01683(11)  .      1_555  N
  N1        Li             2.01683(11)  .      5_555  N
  O2        Sr              2.7233(11)  .      1_655  N
  O2        Sr              2.9801(12)  .      2_655  N
  O2        Sr              2.7233(11)  .      5_654  N
  O2        Sr              2.9801(12)  .      6_654  N
  O2        Ta             2.02018(16)  .      1_655  N
  O2        Ta             2.02018(16)  .    105_555  N
  O2        Li             2.02018(16)  .      1_655  N
  O2        Li             2.02018(16)  .    105_555  N
  N2        Sr              2.7233(11)  .      1_655  N
  N2        Sr              2.9801(12)  .      2_655  N
  N2        Sr              2.7233(11)  .      5_654  N
  N2        Sr              2.9801(12)  .      6_654  N
  N2        Ta             2.02018(16)  .      1_655  N
  N2        Ta             2.02018(16)  .    105_555  N
  N2        Li             2.02018(16)  .      1_655  N
  N2        Li             2.02018(16)  .    105_555  N

loop_
      _geom_angle_atom_site_label_1
      _geom_angle_atom_site_label_2
      _geom_angle_atom_site_label_3
      _geom_angle
      _geom_angle_site_symmetry_1
      _geom_angle_site_symmetry_2
      _geom_angle_site_symmetry_3
      _geom_angle_publ_flag
  Sr        Sr        Sr                    90.0      2_555  .      2_565  N
  Sr        Sr        Sr                    90.0      2_555  .      2_655  N
  Sr        Sr        Sr                   180.0      2_555  .      2_665  N
  Sr        Sr        Sr                    90.0      2_555  .      5_554  N
  Sr        Sr        Sr                    90.0      2_555  .      5_555  N
  Sr        Sr        Ta              54.7682(8)      2_555  .      1_555  N
  Sr        Sr        Ta             125.2318(8)      2_555  .      1_565  N
  Sr        Sr        Ta              54.7682(8)      2_555  .      5_555  N
  Sr        Sr        Ta             125.2318(8)      2_555  .      5_565  N
  Sr        Sr        Ta              54.7682(8)      2_555  .    101_455  N
  Sr        Sr        Ta             125.2318(8)      2_555  .    101_555  N
  Sr        Sr        Ta              54.7682(8)      2_555  .    105_453  N
  Sr        Sr        Ta             125.2318(8)      2_555  .    105_553  N
  Sr        Sr        Li              54.7682(8)      2_555  .      1_555  N
  Sr        Sr        Li             125.2318(8)      2_555  .      1_565  N
  Sr        Sr        Li              54.7682(8)      2_555  .      5_555  N
  Sr        Sr        Li             125.2318(8)      2_555  .      5_565  N
  Sr        Sr        Li              54.7682(8)      2_555  .    101_455  N
  Sr        Sr        Li             125.2318(8)      2_555  .    101_555  N
  Sr        Sr        Li              54.7682(8)      2_555  .    105_453  N
  Sr        Sr        Li             125.2318(8)      2_555  .    105_553  N
  Sr        Sr        O1                    45.0      2_555  .      1_555  N
  Sr        Sr        O1                   135.0      2_555  .      1_565  N
  Sr        Sr        O1                    45.0      2_555  .    105_453  N
  Sr        Sr        Sr                   180.0      2_565  .      2_655  N
  Sr        Sr        Sr                    90.0      2_565  .      2_665  N
  Sr        Sr        Sr                    90.0      2_565  .      5_554  N
  Sr        Sr        Sr                    90.0      2_565  .      5_555  N
  Sr        Sr        Ta             125.2318(8)      2_565  .      1_555  N
  Sr        Sr        Ta              54.7682(8)      2_565  .      1_565  N
  Sr        Sr        Ta             125.2318(8)      2_565  .      5_555  N
  Sr        Sr        Ta              54.7682(8)      2_565  .      5_565  N
  Sr        Sr        Ta              54.7682(8)      2_565  .    101_455  N
  Sr        Sr        Ta             125.2318(8)      2_565  .    101_555  N
  Sr        Sr        Ta              54.7682(8)      2_565  .    105_453  N
  Sr        Sr        Ta             125.2318(8)      2_565  .    105_553  N
  Sr        Sr        Li             125.2318(8)      2_565  .      1_555  N
  Sr        Sr        Li              54.7682(8)      2_565  .      1_565  N
  Sr        Sr        Li             125.2318(8)      2_565  .      5_555  N
  Sr        Sr        Li              54.7682(8)      2_565  .      5_565  N
  Sr        Sr        Li              54.7682(8)      2_565  .    101_455  N
  Sr        Sr        Li             125.2318(8)      2_565  .    101_555  N
  Sr        Sr        Li              54.7682(8)      2_565  .    105_453  N
  Sr        Sr        Li             125.2318(8)      2_565  .    105_553  N
  Sr        Sr        O1                   135.0      2_565  .      1_555  N
  Sr        Sr        O1                    45.0      2_565  .      1_565  N
  Sr        Sr        O1                    45.0      2_565  .    105_453  N
  Sr        Sr        Sr                    90.0      2_655  .      2_665  N
  Sr        Sr        Sr                    90.0      2_655  .      5_554  N
  Sr        Sr        Sr                    90.0      2_655  .      5_555  N
  Sr        Sr        Ta              54.7682(8)      2_655  .      1_555  N
  Sr        Sr        Ta             125.2318(8)      2_655  .      1_565  N
  Sr        Sr        Ta              54.7682(8)      2_655  .      5_555  N
  Sr        Sr        Ta             125.2318(8)      2_655  .      5_565  N
  Sr        Sr        Ta             125.2318(8)      2_655  .    101_455  N
  Sr        Sr        Ta              54.7682(8)      2_655  .    101_555  N
  Sr        Sr        Ta             125.2318(8)      2_655  .    105_453  N
  Sr        Sr        Ta              54.7682(8)      2_655  .    105_553  N
  Sr        Sr        Li              54.7682(8)      2_655  .      1_555  N
  Sr        Sr        Li             125.2318(8)      2_655  .      1_565  N
  Sr        Sr        Li              54.7682(8)      2_655  .      5_555  N
  Sr        Sr        Li             125.2318(8)      2_655  .      5_565  N
  Sr        Sr        Li             125.2318(8)      2_655  .    101_455  N
  Sr        Sr        Li              54.7682(8)      2_655  .    101_555  N
  Sr        Sr        Li             125.2318(8)      2_655  .    105_453  N
  Sr        Sr        Li              54.7682(8)      2_655  .    105_553  N
  Sr        Sr        O1                    45.0      2_655  .      1_555  N
  Sr        Sr        O1                   135.0      2_655  .      1_565  N
  Sr        Sr        O1                   135.0      2_655  .    105_453  N
  Sr        Sr        Sr                    90.0      2_665  .      5_554  N
  Sr        Sr        Sr                    90.0      2_665  .      5_555  N
  Sr        Sr        Ta             125.2318(8)      2_665  .      1_555  N
  Sr        Sr        Ta              54.7682(8)      2_665  .      1_565  N
  Sr        Sr        Ta             125.2318(8)      2_665  .      5_555  N
  Sr        Sr        Ta              54.7682(8)      2_665  .      5_565  N
  Sr        Sr        Ta             125.2318(8)      2_665  .    101_455  N
  Sr        Sr        Ta              54.7682(8)      2_665  .    101_555  N
  Sr        Sr        Ta             125.2318(8)      2_665  .    105_453  N
  Sr        Sr        Ta              54.7682(8)      2_665  .    105_553  N
  Sr        Sr        Li             125.2318(8)      2_665  .      1_555  N
  Sr        Sr        Li              54.7682(8)      2_665  .      1_565  N
  Sr        Sr        Li             125.2318(8)      2_665  .      5_555  N
  Sr        Sr        Li              54.7682(8)      2_665  .      5_565  N
  Sr        Sr        Li             125.2318(8)      2_665  .    101_455  N
  Sr        Sr        Li              54.7682(8)      2_665  .    101_555  N
  Sr        Sr        Li             125.2318(8)      2_665  .    105_453  N
  Sr        Sr        Li              54.7682(8)      2_665  .    105_553  N
  Sr        Sr        O1                   135.0      2_665  .      1_555  N
  Sr        Sr        O1                    45.0      2_665  .      1_565  N
  Sr        Sr        O1                   135.0      2_665  .    105_453  N
  Sr        Sr        Sr                   180.0      5_554  .      5_555  N
  Sr        Sr        Ta             54.6705(17)      5_554  .      1_555  N
  Sr        Sr        Ta             54.6705(17)      5_554  .      1_565  N
  Sr        Sr        Ta            125.3295(17)      5_554  .      5_555  N
  Sr        Sr        Ta            125.3295(17)      5_554  .      5_565  N
  Sr        Sr        Ta            125.3295(17)      5_554  .    101_455  N
  Sr        Sr        Ta            125.3295(17)      5_554  .    101_555  N
  Sr        Sr        Ta             54.6705(17)      5_554  .    105_453  N
  Sr        Sr        Ta             54.6705(17)      5_554  .    105_553  N
  Sr        Sr        Li             54.6705(17)      5_554  .      1_555  N
  Sr        Sr        Li             54.6705(17)      5_554  .      1_565  N
  Sr        Sr        Li            125.3295(17)      5_554  .      5_555  N
  Sr        Sr        Li            125.3295(17)      5_554  .      5_565  N
  Sr        Sr        Li            125.3295(17)      5_554  .    101_455  N
  Sr        Sr        Li            125.3295(17)      5_554  .    101_555  N
  Sr        Sr        Li             54.6705(17)      5_554  .    105_453  N
  Sr        Sr        Li             54.6705(17)      5_554  .    105_553  N
  Sr        Sr        O1                    90.0      5_554  .      1_555  N
  Sr        Sr        O1                    90.0      5_554  .      1_565  N
  Sr        Sr        O1                    90.0      5_554  .    105_453  N
  Sr        Sr        Ta            125.3295(17)      5_555  .      1_555  N
  Sr        Sr        Ta            125.3295(17)      5_555  .      1_565  N
  Sr        Sr        Ta             54.6705(17)      5_555  .      5_555  N
  Sr        Sr        Ta             54.6705(17)      5_555  .      5_565  N
  Sr        Sr        Ta             54.6705(17)      5_555  .    101_455  N
  Sr        Sr        Ta             54.6705(17)      5_555  .    101_555  N
  Sr        Sr        Ta            125.3295(17)      5_555  .    105_453  N
  Sr        Sr        Ta            125.3295(17)      5_555  .    105_553  N
  Sr        Sr        Li            125.3295(17)      5_555  .      1_555  N
  Sr        Sr        Li            125.3295(17)      5_555  .      1_565  N
  Sr        Sr        Li             54.6705(17)      5_555  .      5_555  N
  Sr        Sr        Li             54.6705(17)      5_555  .      5_565  N
  Sr        Sr        Li             54.6705(17)      5_555  .    101_455  N
  Sr        Sr        Li             54.6705(17)      5_555  .    101_555  N
  Sr        Sr        Li            125.3295(17)      5_555  .    105_453  N
  Sr        Sr        Li            125.3295(17)      5_555  .    105_553  N
  Sr        Sr        O1                    90.0      5_555  .      1_555  N
  Sr        Sr        O1                    90.0      5_555  .      1_565  N
  Sr        Sr        O1                    90.0      5_555  .    105_453  N
  Ta        Sr        Ta            109.3409(34)      1_555  .      1_565  N
  Ta        Sr        Ta             70.6591(34)      1_555  .      5_555  N
  Ta        Sr        Ta                   180.0      1_555  .      5_565  N
  Ta        Sr        Ta            109.5364(17)      1_555  .    101_455  N
  Ta        Sr        Ta            109.5364(17)      1_555  .    101_555  N
  Ta        Sr        Ta             70.4636(17)      1_555  .    105_453  N
  Ta        Sr        Ta             70.4636(17)      1_555  .    105_553  N
  Ta        Sr        Li                     0.0      1_555  .      1_555  N
  Ta        Sr        Li            109.3409(34)      1_555  .      1_565  N
  Ta        Sr        Li             70.6591(34)      1_555  .      5_555  N
  Ta        Sr        Li                   180.0      1_555  .      5_565  N
  Ta        Sr        Li            109.5364(17)      1_555  .    101_455  N
  Ta        Sr        Li            109.5364(17)      1_555  .    101_555  N
  Ta        Sr        Li             70.4636(17)      1_555  .    105_453  N
  Ta        Sr        Li             70.4636(17)      1_555  .    105_553  N
  Ta        Sr        O1             35.3295(17)      1_555  .      1_555  N
  Ta        Sr        O1            144.6705(17)      1_555  .      1_565  N
  Ta        Sr        O1                    90.0      1_555  .    105_453  N
  Ta        Sr        Ta                   180.0      1_565  .      5_555  N
  Ta        Sr        Ta             70.6591(34)      1_565  .      5_565  N
  Ta        Sr        Ta            109.5364(17)      1_565  .    101_455  N
  Ta        Sr        Ta            109.5364(17)      1_565  .    101_555  N
  Ta        Sr        Ta             70.4636(17)      1_565  .    105_453  N
  Ta        Sr        Ta             70.4636(17)      1_565  .    105_553  N
  Ta        Sr        Li            109.3409(34)      1_565  .      1_555  N
  Ta        Sr        Li                     0.0      1_565  .      1_565  N
  Ta        Sr        Li                   180.0      1_565  .      5_555  N
  Ta        Sr        Li             70.6591(34)      1_565  .      5_565  N
  Ta        Sr        Li            109.5364(17)      1_565  .    101_455  N
  Ta        Sr        Li            109.5364(17)      1_565  .    101_555  N
  Ta        Sr        Li             70.4636(17)      1_565  .    105_453  N
  Ta        Sr        Li             70.4636(17)      1_565  .    105_553  N
  Ta        Sr        O1            144.6705(17)      1_565  .      1_555  N
  Ta        Sr        O1             35.3295(17)      1_565  .      1_565  N
  Ta        Sr        O1                    90.0      1_565  .    105_453  N
  Ta        Sr        Ta            109.3409(34)      5_555  .      5_565  N
  Ta        Sr        Ta             70.4636(17)      5_555  .    101_455  N
  Ta        Sr        Ta             70.4636(17)      5_555  .    101_555  N
  Ta        Sr        Ta            109.5364(17)      5_555  .    105_453  N
  Ta        Sr        Ta            109.5364(17)      5_555  .    105_553  N
  Ta        Sr        Li             70.6591(34)      5_555  .      1_555  N
  Ta        Sr        Li                   180.0      5_555  .      1_565  N
  Ta        Sr        Li                     0.0      5_555  .      5_555  N
  Ta        Sr        Li            109.3409(34)      5_555  .      5_565  N
  Ta        Sr        Li             70.4636(17)      5_555  .    101_455  N
  Ta        Sr        Li             70.4636(17)      5_555  .    101_555  N
  Ta        Sr        Li            109.5364(17)      5_555  .    105_453  N
  Ta        Sr        Li            109.5364(17)      5_555  .    105_553  N
  Ta        Sr        O1             35.3295(17)      5_555  .      1_555  N
  Ta        Sr        O1            144.6705(17)      5_555  .      1_565  N
  Ta        Sr        O1                    90.0      5_555  .    105_453  N
  Ta        Sr        Ta             70.4636(17)      5_565  .    101_455  N
  Ta        Sr        Ta             70.4636(17)      5_565  .    101_555  N
  Ta        Sr        Ta            109.5364(17)      5_565  .    105_453  N
  Ta        Sr        Ta            109.5364(17)      5_565  .    105_553  N
  Ta        Sr        Li                   180.0      5_565  .      1_555  N
  Ta        Sr        Li             70.6591(34)      5_565  .      1_565  N
  Ta        Sr        Li            109.3409(34)      5_565  .      5_555  N
  Ta        Sr        Li                     0.0      5_565  .      5_565  N
  Ta        Sr        Li             70.4636(17)      5_565  .    101_455  N
  Ta        Sr        Li             70.4636(17)      5_565  .    101_555  N
  Ta        Sr        Li            109.5364(17)      5_565  .    105_453  N
  Ta        Sr        Li            109.5364(17)      5_565  .    105_553  N
  Ta        Sr        O1            144.6705(17)      5_565  .      1_555  N
  Ta        Sr        O1             35.3295(17)      5_565  .      1_565  N
  Ta        Sr        O1                    90.0      5_565  .    105_453  N
  Ta        Sr        Ta            109.3409(34)    101_455  .    101_555  N
  Ta        Sr        Ta             70.6591(34)    101_455  .    105_453  N
  Ta        Sr        Ta                   180.0    101_455  .    105_553  N
  Ta        Sr        Li            109.5364(17)    101_455  .      1_555  N
  Ta        Sr        Li            109.5364(17)    101_455  .      1_565  N
  Ta        Sr        Li             70.4636(17)    101_455  .      5_555  N
  Ta        Sr        Li             70.4636(17)    101_455  .      5_565  N
  Ta        Sr        Li                     0.0    101_455  .    101_455  N
  Ta        Sr        Li            109.3409(34)    101_455  .    101_555  N
  Ta        Sr        Li             70.6591(34)    101_455  .    105_453  N
  Ta        Sr        Li                   180.0    101_455  .    105_553  N
  Ta        Sr        O1                    90.0    101_455  .      1_555  N
  Ta        Sr        O1                    90.0    101_455  .      1_565  N
  Ta        Sr        O1             35.3295(17)    101_455  .    105_453  N
  Ta        Sr        Ta                   180.0    101_555  .    105_453  N
  Ta        Sr        Ta             70.6591(34)    101_555  .    105_553  N
  Ta        Sr        Li            109.5364(17)    101_555  .      1_555  N
  Ta        Sr        Li            109.5364(17)    101_555  .      1_565  N
  Ta        Sr        Li             70.4636(17)    101_555  .      5_555  N
  Ta        Sr        Li             70.4636(17)    101_555  .      5_565  N
  Ta        Sr        Li            109.3409(34)    101_555  .    101_455  N
  Ta        Sr        Li                     0.0    101_555  .    101_555  N
  Ta        Sr        Li                   180.0    101_555  .    105_453  N
  Ta        Sr        Li             70.6591(34)    101_555  .    105_553  N
  Ta        Sr        O1                    90.0    101_555  .      1_555  N
  Ta        Sr        O1                    90.0    101_555  .      1_565  N
  Ta        Sr        O1            144.6705(17)    101_555  .    105_453  N
  Ta        Sr        Ta            109.3409(34)    105_453  .    105_553  N
  Ta        Sr        Li             70.4636(17)    105_453  .      1_555  N
  Ta        Sr        Li             70.4636(17)    105_453  .      1_565  N
  Ta        Sr        Li            109.5364(17)    105_453  .      5_555  N
  Ta        Sr        Li            109.5364(17)    105_453  .      5_565  N
  Ta        Sr        Li             70.6591(34)    105_453  .    101_455  N
  Ta        Sr        Li                   180.0    105_453  .    101_555  N
  Ta        Sr        Li                     0.0    105_453  .    105_453  N
  Ta        Sr        Li            109.3409(34)    105_453  .    105_553  N
  Ta        Sr        O1                    90.0    105_453  .      1_555  N
  Ta        Sr        O1                    90.0    105_453  .      1_565  N
  Ta        Sr        O1             35.3295(17)    105_453  .    105_453  N
  Ta        Sr        Li             70.4636(17)    105_553  .      1_555  N
  Ta        Sr        Li             70.4636(17)    105_553  .      1_565  N
  Ta        Sr        Li            109.5364(17)    105_553  .      5_555  N
  Ta        Sr        Li            109.5364(17)    105_553  .      5_565  N
  Ta        Sr        Li                   180.0    105_553  .    101_455  N
  Ta        Sr        Li             70.6591(34)    105_553  .    101_555  N
  Ta        Sr        Li            109.3409(34)    105_553  .    105_453  N
  Ta        Sr        Li                     0.0    105_553  .    105_553  N
  Ta        Sr        O1                    90.0    105_553  .      1_555  N
  Ta        Sr        O1                    90.0    105_553  .      1_565  N
  Ta        Sr        O1            144.6705(17)    105_553  .    105_453  N
  Li        Sr        Li            109.3409(34)      1_555  .      1_565  N
  Li        Sr        Li             70.6591(34)      1_555  .      5_555  N
  Li        Sr        Li                   180.0      1_555  .      5_565  N
  Li        Sr        Li            109.5364(17)      1_555  .    101_455  N
  Li        Sr        Li            109.5364(17)      1_555  .    101_555  N
  Li        Sr        Li             70.4636(17)      1_555  .    105_453  N
  Li        Sr        Li             70.4636(17)      1_555  .    105_553  N
  Li        Sr        O1             35.3295(17)      1_555  .      1_555  N
  Li        Sr        O1            144.6705(17)      1_555  .      1_565  N
  Li        Sr        O1                    90.0      1_555  .    105_453  N
  Li        Sr        Li                   180.0      1_565  .      5_555  N
  Li        Sr        Li             70.6591(34)      1_565  .      5_565  N
  Li        Sr        Li            109.5364(17)      1_565  .    101_455  N
  Li        Sr        Li            109.5364(17)      1_565  .    101_555  N
  Li        Sr        Li             70.4636(17)      1_565  .    105_453  N
  Li        Sr        Li             70.4636(17)      1_565  .    105_553  N
  Li        Sr        O1            144.6705(17)      1_565  .      1_555  N
  Li        Sr        O1             35.3295(17)      1_565  .      1_565  N
  Li        Sr        O1                    90.0      1_565  .    105_453  N
  Li        Sr        Li            109.3409(34)      5_555  .      5_565  N
  Li        Sr        Li             70.4636(17)      5_555  .    101_455  N
  Li        Sr        Li             70.4636(17)      5_555  .    101_555  N
  Li        Sr        Li            109.5364(17)      5_555  .    105_453  N
  Li        Sr        Li            109.5364(17)      5_555  .    105_553  N
  Li        Sr        O1             35.3295(17)      5_555  .      1_555  N
  Li        Sr        O1            144.6705(17)      5_555  .      1_565  N
  Li        Sr        O1                    90.0      5_555  .    105_453  N
  Li        Sr        Li             70.4636(17)      5_565  .    101_455  N
  Li        Sr        Li             70.4636(17)      5_565  .    101_555  N
  Li        Sr        Li            109.5364(17)      5_565  .    105_453  N
  Li        Sr        Li            109.5364(17)      5_565  .    105_553  N
  Li        Sr        O1            144.6705(17)      5_565  .      1_555  N
  Li        Sr        O1             35.3295(17)      5_565  .      1_565  N
  Li        Sr        O1                    90.0      5_565  .    105_453  N
  Li        Sr        Li            109.3409(34)    101_455  .    101_555  N
  Li        Sr        Li             70.6591(34)    101_455  .    105_453  N
  Li        Sr        Li                   180.0    101_455  .    105_553  N
  Li        Sr        O1                    90.0    101_455  .      1_555  N
  Li        Sr        O1                    90.0    101_455  .      1_565  N
  Li        Sr        O1             35.3295(17)    101_455  .    105_453  N
  Li        Sr        Li                   180.0    101_555  .    105_453  N
  Li        Sr        Li             70.6591(34)    101_555  .    105_553  N
  Li        Sr        O1                    90.0    101_555  .      1_555  N
  Li        Sr        O1                    90.0    101_555  .      1_565  N
  Li        Sr        O1            144.6705(17)    101_555  .    105_453  N
  Li        Sr        Li            109.3409(34)    105_453  .    105_553  N
  Li        Sr        O1                    90.0    105_453  .      1_555  N
  Li        Sr        O1                    90.0    105_453  .      1_565  N
  Li        Sr        O1             35.3295(17)    105_453  .    105_453  N
  Li        Sr        O1                    90.0    105_553  .      1_555  N
  Li        Sr        O1                    90.0    105_553  .      1_565  N
  Li        Sr        O1            144.6705(17)    105_553  .    105_453  N
  O1        Sr        O1                   180.0      1_555  .      1_565  N
  O1        Sr        O1                    90.0      1_555  .    105_453  N
  O1        Sr        O1                    90.0      1_565  .    105_453  N
  Sr        Ta        Sr            109.3409(34)      1_545  .      1_555  N
  Sr        Ta        Sr             70.4636(17)      1_545  .      2_555  N
  Sr        Ta        Sr             70.4636(17)      1_545  .      2_655  N
  Sr        Ta        Sr             70.6591(34)      1_545  .      5_544  N
  Sr        Ta        Sr                   180.0      1_545  .      5_554  N
  Sr        Ta        Sr            109.5364(17)      1_545  .      6_554  N
  Sr        Ta        Sr            109.5364(17)      1_545  .      6_654  N
  Sr        Ta        O1             54.6705(17)      1_545  .      1_555  N
  Sr        Ta        O1            125.3295(17)      1_545  .      5_554  N
  Sr        Ta        N1             54.6705(17)      1_545  .      1_555  N
  Sr        Ta        N1            125.3295(17)      1_545  .      5_554  N
  Sr        Ta        O2             128.794(31)      1_545  .      1_455  N
  Sr        Ta        O2              58.496(34)      1_545  .      2_545  N
  Sr        Ta        O2              51.207(31)      1_545  .      3_655  N
  Sr        Ta        O2             121.504(34)      1_545  .      4_565  N
  Sr        Ta        N2             128.794(31)      1_545  .      1_455  N
  Sr        Ta        N2              58.496(34)      1_545  .      2_545  N
  Sr        Ta        N2              51.207(31)      1_545  .      3_655  N
  Sr        Ta        N2             121.504(34)      1_545  .      4_565  N
  Sr        Ta        Sr             70.4636(17)      1_555  .      2_555  N
  Sr        Ta        Sr             70.4636(17)      1_555  .      2_655  N
  Sr        Ta        Sr                   180.0      1_555  .      5_544  N
  Sr        Ta        Sr             70.6591(34)      1_555  .      5_554  N
  Sr        Ta        Sr            109.5364(17)      1_555  .      6_554  N
  Sr        Ta        Sr            109.5364(17)      1_555  .      6_654  N
  Sr        Ta        O1             54.6705(17)      1_555  .      1_555  N
  Sr        Ta        O1            125.3295(17)      1_555  .      5_554  N
  Sr        Ta        N1             54.6705(17)      1_555  .      1_555  N
  Sr        Ta        N1            125.3295(17)      1_555  .      5_554  N
  Sr        Ta        O2              51.207(31)      1_555  .      1_455  N
  Sr        Ta        O2             121.504(34)      1_555  .      2_545  N
  Sr        Ta        O2             128.794(31)      1_555  .      3_655  N
  Sr        Ta        O2              58.496(34)      1_555  .      4_565  N
  Sr        Ta        N2              51.207(31)      1_555  .      1_455  N
  Sr        Ta        N2             121.504(34)      1_555  .      2_545  N
  Sr        Ta        N2             128.794(31)      1_555  .      3_655  N
  Sr        Ta        N2              58.496(34)      1_555  .      4_565  N
  Sr        Ta        Sr            109.3409(34)      2_555  .      2_655  N
  Sr        Ta        Sr            109.5364(17)      2_555  .      5_544  N
  Sr        Ta        Sr            109.5364(17)      2_555  .      5_554  N
  Sr        Ta        Sr             70.6591(34)      2_555  .      6_554  N
  Sr        Ta        Sr                   180.0      2_555  .      6_654  N
  Sr        Ta        O1             54.6705(17)      2_555  .      1_555  N
  Sr        Ta        O1            125.3295(17)      2_555  .      5_554  N
  Sr        Ta        N1             54.6705(17)      2_555  .      1_555  N
  Sr        Ta        N1            125.3295(17)      2_555  .      5_554  N
  Sr        Ta        O2              58.496(34)      2_555  .      1_455  N
  Sr        Ta        O2              51.207(31)      2_555  .      2_545  N
  Sr        Ta        O2             121.504(34)      2_555  .      3_655  N
  Sr        Ta        O2             128.794(31)      2_555  .      4_565  N
  Sr        Ta        N2              58.496(34)      2_555  .      1_455  N
  Sr        Ta        N2              51.207(31)      2_555  .      2_545  N
  Sr        Ta        N2             121.504(34)      2_555  .      3_655  N
  Sr        Ta        N2             128.794(31)      2_555  .      4_565  N
  Sr        Ta        Sr            109.5364(17)      2_655  .      5_544  N
  Sr        Ta        Sr            109.5364(17)      2_655  .      5_554  N
  Sr        Ta        Sr                   180.0      2_655  .      6_554  N
  Sr        Ta        Sr             70.6591(34)      2_655  .      6_654  N
  Sr        Ta        O1             54.6705(17)      2_655  .      1_555  N
  Sr        Ta        O1            125.3295(17)      2_655  .      5_554  N
  Sr        Ta        N1             54.6705(17)      2_655  .      1_555  N
  Sr        Ta        N1            125.3295(17)      2_655  .      5_554  N
  Sr        Ta        O2             121.504(34)      2_655  .      1_455  N
  Sr        Ta        O2             128.794(31)      2_655  .      2_545  N
  Sr        Ta        O2              58.496(34)      2_655  .      3_655  N
  Sr        Ta        O2              51.207(31)      2_655  .      4_565  N
  Sr        Ta        N2             121.504(34)      2_655  .      1_455  N
  Sr        Ta        N2             128.794(31)      2_655  .      2_545  N
  Sr        Ta        N2              58.496(34)      2_655  .      3_655  N
  Sr        Ta        N2              51.207(31)      2_655  .      4_565  N
  Sr        Ta        Sr            109.3409(34)      5_544  .      5_554  N
  Sr        Ta        Sr             70.4636(17)      5_544  .      6_554  N
  Sr        Ta        Sr             70.4636(17)      5_544  .      6_654  N
  Sr        Ta        O1            125.3295(17)      5_544  .      1_555  N
  Sr        Ta        O1             54.6705(17)      5_544  .      5_554  N
  Sr        Ta        N1            125.3295(17)      5_544  .      1_555  N
  Sr        Ta        N1             54.6705(17)      5_544  .      5_554  N
  Sr        Ta        O2             128.794(31)      5_544  .      1_455  N
  Sr        Ta        O2              58.496(34)      5_544  .      2_545  N
  Sr        Ta        O2              51.207(31)      5_544  .      3_655  N
  Sr        Ta        O2             121.504(34)      5_544  .      4_565  N
  Sr        Ta        N2             128.794(31)      5_544  .      1_455  N
  Sr        Ta        N2              58.496(34)      5_544  .      2_545  N
  Sr        Ta        N2              51.207(31)      5_544  .      3_655  N
  Sr        Ta        N2             121.504(34)      5_544  .      4_565  N
  Sr        Ta        Sr             70.4636(17)      5_554  .      6_554  N
  Sr        Ta        Sr             70.4636(17)      5_554  .      6_654  N
  Sr        Ta        O1            125.3295(17)      5_554  .      1_555  N
  Sr        Ta        O1             54.6705(17)      5_554  .      5_554  N
  Sr        Ta        N1            125.3295(17)      5_554  .      1_555  N
  Sr        Ta        N1             54.6705(17)      5_554  .      5_554  N
  Sr        Ta        O2              51.207(31)      5_554  .      1_455  N
  Sr        Ta        O2             121.504(34)      5_554  .      2_545  N
  Sr        Ta        O2             128.794(31)      5_554  .      3_655  N
  Sr        Ta        O2              58.496(34)      5_554  .      4_565  N
  Sr        Ta        N2              51.207(31)      5_554  .      1_455  N
  Sr        Ta        N2             121.504(34)      5_554  .      2_545  N
  Sr        Ta        N2             128.794(31)      5_554  .      3_655  N
  Sr        Ta        N2              58.496(34)      5_554  .      4_565  N
  Sr        Ta        Sr            109.3409(34)      6_554  .      6_654  N
  Sr        Ta        O1            125.3295(17)      6_554  .      1_555  N
  Sr        Ta        O1             54.6705(17)      6_554  .      5_554  N
  Sr        Ta        N1            125.3295(17)      6_554  .      1_555  N
  Sr        Ta        N1             54.6705(17)      6_554  .      5_554  N
  Sr        Ta        O2              58.496(34)      6_554  .      1_455  N
  Sr        Ta        O2              51.207(31)      6_554  .      2_545  N
  Sr        Ta        O2             121.504(34)      6_554  .      3_655  N
  Sr        Ta        O2             128.794(31)      6_554  .      4_565  N
  Sr        Ta        N2              58.496(34)      6_554  .      1_455  N
  Sr        Ta        N2              51.207(31)      6_554  .      2_545  N
  Sr        Ta        N2             121.504(34)      6_554  .      3_655  N
  Sr        Ta        N2             128.794(31)      6_554  .      4_565  N
  Sr        Ta        O1            125.3295(17)      6_654  .      1_555  N
  Sr        Ta        O1             54.6705(17)      6_654  .      5_554  N
  Sr        Ta        N1            125.3295(17)      6_654  .      1_555  N
  Sr        Ta        N1             54.6705(17)      6_654  .      5_554  N
  Sr        Ta        O2             121.504(34)      6_654  .      1_455  N
  Sr        Ta        O2             128.794(31)      6_654  .      2_545  N
  Sr        Ta        O2              58.496(34)      6_654  .      3_655  N
  Sr        Ta        O2              51.207(31)      6_654  .      4_565  N
  Sr        Ta        N2             121.504(34)      6_654  .      1_455  N
  Sr        Ta        N2             128.794(31)      6_654  .      2_545  N
  Sr        Ta        N2              58.496(34)      6_654  .      3_655  N
  Sr        Ta        N2              51.207(31)      6_654  .      4_565  N
  O1        Ta        O1                   180.0      1_555  .      5_554  N
  O1        Ta        N1                     0.0      1_555  .      1_555  N
  O1        Ta        N1                   180.0      1_555  .      5_554  N
  O1        Ta        O2                    90.0      1_555  .      1_455  N
  O1        Ta        O2                    90.0      1_555  .      2_545  N
  O1        Ta        O2                    90.0      1_555  .      3_655  N
  O1        Ta        O2                    90.0      1_555  .      4_565  N
  O1        Ta        N2                    90.0      1_555  .      1_455  N
  O1        Ta        N2                    90.0      1_555  .      2_545  N
  O1        Ta        N2                    90.0      1_555  .      3_655  N
  O1        Ta        N2                    90.0      1_555  .      4_565  N
  O1        Ta        N1                   180.0      5_554  .      1_555  N
  O1        Ta        N1                     0.0      5_554  .      5_554  N
  O1        Ta        O2                    90.0      5_554  .      1_455  N
  O1        Ta        O2                    90.0      5_554  .      2_545  N
  O1        Ta        O2                    90.0      5_554  .      3_655  N
  O1        Ta        O2                    90.0      5_554  .      4_565  N
  O1        Ta        N2                    90.0      5_554  .      1_455  N
  O1        Ta        N2                    90.0      5_554  .      2_545  N
  O1        Ta        N2                    90.0      5_554  .      3_655  N
  O1        Ta        N2                    90.0      5_554  .      4_565  N
  N1        Ta        N1                   180.0      1_555  .      5_554  N
  N1        Ta        O2                    90.0      1_555  .      1_455  N
  N1        Ta        O2                    90.0      1_555  .      2_545  N
  N1        Ta        O2                    90.0      1_555  .      3_655  N
  N1        Ta        O2                    90.0      1_555  .      4_565  N
  N1        Ta        N2                    90.0      1_555  .      1_455  N
  N1        Ta        N2                    90.0      1_555  .      2_545  N
  N1        Ta        N2                    90.0      1_555  .      3_655  N
  N1        Ta        N2                    90.0      1_555  .      4_565  N
  N1        Ta        O2                    90.0      5_554  .      1_455  N
  N1        Ta        O2                    90.0      5_554  .      2_545  N
  N1        Ta        O2                    90.0      5_554  .      3_655  N
  N1        Ta        O2                    90.0      5_554  .      4_565  N
  N1        Ta        N2                    90.0      5_554  .      1_455  N
  N1        Ta        N2                    90.0      5_554  .      2_545  N
  N1        Ta        N2                    90.0      5_554  .      3_655  N
  N1        Ta        N2                    90.0      5_554  .      4_565  N
  O2        Ta        O2                    90.0      1_455  .      2_545  N
  O2        Ta        O2                   180.0      1_455  .      3_655  N
  O2        Ta        O2                    90.0      1_455  .      4_565  N
  O2        Ta        N2                     0.0      1_455  .      1_455  N
  O2        Ta        N2                    90.0      1_455  .      2_545  N
  O2        Ta        N2                   180.0      1_455  .      3_655  N
  O2        Ta        N2                    90.0      1_455  .      4_565  N
  O2        Ta        O2                    90.0      2_545  .      3_655  N
  O2        Ta        O2                   180.0      2_545  .      4_565  N
  O2        Ta        N2                    90.0      2_545  .      1_455  N
  O2        Ta        N2                     0.0      2_545  .      2_545  N
  O2        Ta        N2                    90.0      2_545  .      3_655  N
  O2        Ta        N2                   180.0      2_545  .      4_565  N
  O2        Ta        O2                    90.0      3_655  .      4_565  N
  O2        Ta        N2                   180.0      3_655  .      1_455  N
  O2        Ta        N2                    90.0      3_655  .      2_545  N
  O2        Ta        N2                     0.0      3_655  .      3_655  N
  O2        Ta        N2                    90.0      3_655  .      4_565  N
  O2        Ta        N2                    90.0      4_565  .      1_455  N
  O2        Ta        N2                   180.0      4_565  .      2_545  N
  O2        Ta        N2                    90.0      4_565  .      3_655  N
  O2        Ta        N2                     0.0      4_565  .      4_565  N
  N2        Ta        N2                    90.0      1_455  .      2_545  N
  N2        Ta        N2                   180.0      1_455  .      3_655  N
  N2        Ta        N2                    90.0      1_455  .      4_565  N
  N2        Ta        N2                    90.0      2_545  .      3_655  N
  N2        Ta        N2                   180.0      2_545  .      4_565  N
  N2        Ta        N2                    90.0      3_655  .      4_565  N
  Sr        Li        Sr            109.3409(34)      1_545  .      1_555  N
  Sr        Li        Sr             70.4636(17)      1_545  .      2_555  N
  Sr        Li        Sr             70.4636(17)      1_545  .      2_655  N
  Sr        Li        Sr             70.6591(34)      1_545  .      5_544  N
  Sr        Li        Sr                   180.0      1_545  .      5_554  N
  Sr        Li        Sr            109.5364(17)      1_545  .      6_554  N
  Sr        Li        Sr            109.5364(17)      1_545  .      6_654  N
  Sr        Li        O1             54.6705(17)      1_545  .      1_555  N
  Sr        Li        O1            125.3295(17)      1_545  .      5_554  N
  Sr        Li        N1             54.6705(17)      1_545  .      1_555  N
  Sr        Li        N1            125.3295(17)      1_545  .      5_554  N
  Sr        Li        O2             128.794(31)      1_545  .      1_455  N
  Sr        Li        O2              58.496(34)      1_545  .      2_545  N
  Sr        Li        O2              51.207(31)      1_545  .      3_655  N
  Sr        Li        O2             121.504(34)      1_545  .      4_565  N
  Sr        Li        N2             128.794(31)      1_545  .      1_455  N
  Sr        Li        N2              58.496(34)      1_545  .      2_545  N
  Sr        Li        N2              51.207(31)      1_545  .      3_655  N
  Sr        Li        N2             121.504(34)      1_545  .      4_565  N
  Sr        Li        Sr             70.4636(17)      1_555  .      2_555  N
  Sr        Li        Sr             70.4636(17)      1_555  .      2_655  N
  Sr        Li        Sr                   180.0      1_555  .      5_544  N
  Sr        Li        Sr             70.6591(34)      1_555  .      5_554  N
  Sr        Li        Sr            109.5364(17)      1_555  .      6_554  N
  Sr        Li        Sr            109.5364(17)      1_555  .      6_654  N
  Sr        Li        O1             54.6705(17)      1_555  .      1_555  N
  Sr        Li        O1            125.3295(17)      1_555  .      5_554  N
  Sr        Li        N1             54.6705(17)      1_555  .      1_555  N
  Sr        Li        N1            125.3295(17)      1_555  .      5_554  N
  Sr        Li        O2              51.207(31)      1_555  .      1_455  N
  Sr        Li        O2             121.504(34)      1_555  .      2_545  N
  Sr        Li        O2             128.794(31)      1_555  .      3_655  N
  Sr        Li        O2              58.496(34)      1_555  .      4_565  N
  Sr        Li        N2              51.207(31)      1_555  .      1_455  N
  Sr        Li        N2             121.504(34)      1_555  .      2_545  N
  Sr        Li        N2             128.794(31)      1_555  .      3_655  N
  Sr        Li        N2              58.496(34)      1_555  .      4_565  N
  Sr        Li        Sr            109.3409(34)      2_555  .      2_655  N
  Sr        Li        Sr            109.5364(17)      2_555  .      5_544  N
  Sr        Li        Sr            109.5364(17)      2_555  .      5_554  N
  Sr        Li        Sr             70.6591(34)      2_555  .      6_554  N
  Sr        Li        Sr                   180.0      2_555  .      6_654  N
  Sr        Li        O1             54.6705(17)      2_555  .      1_555  N
  Sr        Li        O1            125.3295(17)      2_555  .      5_554  N
  Sr        Li        N1             54.6705(17)      2_555  .      1_555  N
  Sr        Li        N1            125.3295(17)      2_555  .      5_554  N
  Sr        Li        O2              58.496(34)      2_555  .      1_455  N
  Sr        Li        O2              51.207(31)      2_555  .      2_545  N
  Sr        Li        O2             121.504(34)      2_555  .      3_655  N
  Sr        Li        O2             128.794(31)      2_555  .      4_565  N
  Sr        Li        N2              58.496(34)      2_555  .      1_455  N
  Sr        Li        N2              51.207(31)      2_555  .      2_545  N
  Sr        Li        N2             121.504(34)      2_555  .      3_655  N
  Sr        Li        N2             128.794(31)      2_555  .      4_565  N
  Sr        Li        Sr            109.5364(17)      2_655  .      5_544  N
  Sr        Li        Sr            109.5364(17)      2_655  .      5_554  N
  Sr        Li        Sr                   180.0      2_655  .      6_554  N
  Sr        Li        Sr             70.6591(34)      2_655  .      6_654  N
  Sr        Li        O1             54.6705(17)      2_655  .      1_555  N
  Sr        Li        O1            125.3295(17)      2_655  .      5_554  N
  Sr        Li        N1             54.6705(17)      2_655  .      1_555  N
  Sr        Li        N1            125.3295(17)      2_655  .      5_554  N
  Sr        Li        O2             121.504(34)      2_655  .      1_455  N
  Sr        Li        O2             128.794(31)      2_655  .      2_545  N
  Sr        Li        O2              58.496(34)      2_655  .      3_655  N
  Sr        Li        O2              51.207(31)      2_655  .      4_565  N
  Sr        Li        N2             121.504(34)      2_655  .      1_455  N
  Sr        Li        N2             128.794(31)      2_655  .      2_545  N
  Sr        Li        N2              58.496(34)      2_655  .      3_655  N
  Sr        Li        N2              51.207(31)      2_655  .      4_565  N
  Sr        Li        Sr            109.3409(34)      5_544  .      5_554  N
  Sr        Li        Sr             70.4636(17)      5_544  .      6_554  N
  Sr        Li        Sr             70.4636(17)      5_544  .      6_654  N
  Sr        Li        O1            125.3295(17)      5_544  .      1_555  N
  Sr        Li        O1             54.6705(17)      5_544  .      5_554  N
  Sr        Li        N1            125.3295(17)      5_544  .      1_555  N
  Sr        Li        N1             54.6705(17)      5_544  .      5_554  N
  Sr        Li        O2             128.794(31)      5_544  .      1_455  N
  Sr        Li        O2              58.496(34)      5_544  .      2_545  N
  Sr        Li        O2              51.207(31)      5_544  .      3_655  N
  Sr        Li        O2             121.504(34)      5_544  .      4_565  N
  Sr        Li        N2             128.794(31)      5_544  .      1_455  N
  Sr        Li        N2              58.496(34)      5_544  .      2_545  N
  Sr        Li        N2              51.207(31)      5_544  .      3_655  N
  Sr        Li        N2             121.504(34)      5_544  .      4_565  N
  Sr        Li        Sr             70.4636(17)      5_554  .      6_554  N
  Sr        Li        Sr             70.4636(17)      5_554  .      6_654  N
  Sr        Li        O1            125.3295(17)      5_554  .      1_555  N
  Sr        Li        O1             54.6705(17)      5_554  .      5_554  N
  Sr        Li        N1            125.3295(17)      5_554  .      1_555  N
  Sr        Li        N1             54.6705(17)      5_554  .      5_554  N
  Sr        Li        O2              51.207(31)      5_554  .      1_455  N
  Sr        Li        O2             121.504(34)      5_554  .      2_545  N
  Sr        Li        O2             128.794(31)      5_554  .      3_655  N
  Sr        Li        O2              58.496(34)      5_554  .      4_565  N
  Sr        Li        N2              51.207(31)      5_554  .      1_455  N
  Sr        Li        N2             121.504(34)      5_554  .      2_545  N
  Sr        Li        N2             128.794(31)      5_554  .      3_655  N
  Sr        Li        N2              58.496(34)      5_554  .      4_565  N
  Sr        Li        Sr            109.3409(34)      6_554  .      6_654  N
  Sr        Li        O1            125.3295(17)      6_554  .      1_555  N
  Sr        Li        O1             54.6705(17)      6_554  .      5_554  N
  Sr        Li        N1            125.3295(17)      6_554  .      1_555  N
  Sr        Li        N1             54.6705(17)      6_554  .      5_554  N
  Sr        Li        O2              58.496(34)      6_554  .      1_455  N
  Sr        Li        O2              51.207(31)      6_554  .      2_545  N
  Sr        Li        O2             121.504(34)      6_554  .      3_655  N
  Sr        Li        O2             128.794(31)      6_554  .      4_565  N
  Sr        Li        N2              58.496(34)      6_554  .      1_455  N
  Sr        Li        N2              51.207(31)      6_554  .      2_545  N
  Sr        Li        N2             121.504(34)      6_554  .      3_655  N
  Sr        Li        N2             128.794(31)      6_554  .      4_565  N
  Sr        Li        O1            125.3295(17)      6_654  .      1_555  N
  Sr        Li        O1             54.6705(17)      6_654  .      5_554  N
  Sr        Li        N1            125.3295(17)      6_654  .      1_555  N
  Sr        Li        N1             54.6705(17)      6_654  .      5_554  N
  Sr        Li        O2             121.504(34)      6_654  .      1_455  N
  Sr        Li        O2             128.794(31)      6_654  .      2_545  N
  Sr        Li        O2              58.496(34)      6_654  .      3_655  N
  Sr        Li        O2              51.207(31)      6_654  .      4_565  N
  Sr        Li        N2             121.504(34)      6_654  .      1_455  N
  Sr        Li        N2             128.794(31)      6_654  .      2_545  N
  Sr        Li        N2              58.496(34)      6_654  .      3_655  N
  Sr        Li        N2              51.207(31)      6_654  .      4_565  N
  O1        Li        O1                   180.0      1_555  .      5_554  N
  O1        Li        N1                     0.0      1_555  .      1_555  N
  O1        Li        N1                   180.0      1_555  .      5_554  N
  O1        Li        O2                    90.0      1_555  .      1_455  N
  O1        Li        O2                    90.0      1_555  .      2_545  N
  O1        Li        O2                    90.0      1_555  .      3_655  N
  O1        Li        O2                    90.0      1_555  .      4_565  N
  O1        Li        N2                    90.0      1_555  .      1_455  N
  O1        Li        N2                    90.0      1_555  .      2_545  N
  O1        Li        N2                    90.0      1_555  .      3_655  N
  O1        Li        N2                    90.0      1_555  .      4_565  N
  O1        Li        N1                   180.0      5_554  .      1_555  N
  O1        Li        N1                     0.0      5_554  .      5_554  N
  O1        Li        O2                    90.0      5_554  .      1_455  N
  O1        Li        O2                    90.0      5_554  .      2_545  N
  O1        Li        O2                    90.0      5_554  .      3_655  N
  O1        Li        O2                    90.0      5_554  .      4_565  N
  O1        Li        N2                    90.0      5_554  .      1_455  N
  O1        Li        N2                    90.0      5_554  .      2_545  N
  O1        Li        N2                    90.0      5_554  .      3_655  N
  O1        Li        N2                    90.0      5_554  .      4_565  N
  N1        Li        N1                   180.0      1_555  .      5_554  N
  N1        Li        O2                    90.0      1_555  .      1_455  N
  N1        Li        O2                    90.0      1_555  .      2_545  N
  N1        Li        O2                    90.0      1_555  .      3_655  N
  N1        Li        O2                    90.0      1_555  .      4_565  N
  N1        Li        N2                    90.0      1_555  .      1_455  N
  N1        Li        N2                    90.0      1_555  .      2_545  N
  N1        Li        N2                    90.0      1_555  .      3_655  N
  N1        Li        N2                    90.0      1_555  .      4_565  N
  N1        Li        O2                    90.0      5_554  .      1_455  N
  N1        Li        O2                    90.0      5_554  .      2_545  N
  N1        Li        O2                    90.0      5_554  .      3_655  N
  N1        Li        O2                    90.0      5_554  .      4_565  N
  N1        Li        N2                    90.0      5_554  .      1_455  N
  N1        Li        N2                    90.0      5_554  .      2_545  N
  N1        Li        N2                    90.0      5_554  .      3_655  N
  N1        Li        N2                    90.0      5_554  .      4_565  N
  O2        Li        O2                    90.0      1_455  .      2_545  N
  O2        Li        O2                   180.0      1_455  .      3_655  N
  O2        Li        O2                    90.0      1_455  .      4_565  N
  O2        Li        N2                     0.0      1_455  .      1_455  N
  O2        Li        N2                    90.0      1_455  .      2_545  N
  O2        Li        N2                   180.0      1_455  .      3_655  N
  O2        Li        N2                    90.0      1_455  .      4_565  N
  O2        Li        O2                    90.0      2_545  .      3_655  N
  O2        Li        O2                   180.0      2_545  .      4_565  N
  O2        Li        N2                    90.0      2_545  .      1_455  N
  O2        Li        N2                     0.0      2_545  .      2_545  N
  O2        Li        N2                    90.0      2_545  .      3_655  N
  O2        Li        N2                   180.0      2_545  .      4_565  N
  O2        Li        O2                    90.0      3_655  .      4_565  N
  O2        Li        N2                   180.0      3_655  .      1_455  N
  O2        Li        N2                    90.0      3_655  .      2_545  N
  O2        Li        N2                     0.0      3_655  .      3_655  N
  O2        Li        N2                    90.0      3_655  .      4_565  N
  O2        Li        N2                    90.0      4_565  .      1_455  N
  O2        Li        N2                   180.0      4_565  .      2_545  N
  O2        Li        N2                    90.0      4_565  .      3_655  N
  O2        Li        N2                     0.0      4_565  .      4_565  N
  N2        Li        N2                    90.0      1_455  .      2_545  N
  N2        Li        N2                   180.0      1_455  .      3_655  N
  N2        Li        N2                    90.0      1_455  .      4_565  N
  N2        Li        N2                    90.0      2_545  .      3_655  N
  N2        Li        N2                   180.0      2_545  .      4_565  N
  N2        Li        N2                    90.0      3_655  .      4_565  N
  Sr        O1        Sr                   180.0      1_545  .      1_555  N
  Sr        O1        Sr                    90.0      1_545  .      2_555  N
  Sr        O1        Sr                    90.0      1_545  .      2_655  N
  Sr        O1        Ta                    90.0      1_545  .      1_555  N
  Sr        O1        Ta                    90.0      1_545  .      5_555  N
  Sr        O1        Li                    90.0      1_545  .      1_555  N
  Sr        O1        Li                    90.0      1_545  .      5_555  N
  Sr        O1        Sr                    90.0      1_555  .      2_555  N
  Sr        O1        Sr                    90.0      1_555  .      2_655  N
  Sr        O1        Ta                    90.0      1_555  .      1_555  N
  Sr        O1        Ta                    90.0      1_555  .      5_555  N
  Sr        O1        Li                    90.0      1_555  .      1_555  N
  Sr        O1        Li                    90.0      1_555  .      5_555  N
  Sr        O1        Sr                   180.0      2_555  .      2_655  N
  Sr        O1        Ta                    90.0      2_555  .      1_555  N
  Sr        O1        Ta                    90.0      2_555  .      5_555  N
  Sr        O1        Li                    90.0      2_555  .      1_555  N
  Sr        O1        Li                    90.0      2_555  .      5_555  N
  Sr        O1        Ta                    90.0      2_655  .      1_555  N
  Sr        O1        Ta                    90.0      2_655  .      5_555  N
  Sr        O1        Li                    90.0      2_655  .      1_555  N
  Sr        O1        Li                    90.0      2_655  .      5_555  N
  Ta        O1        Ta                   180.0      1_555  .      5_555  N
  Ta        O1        Li                     0.0      1_555  .      1_555  N
  Ta        O1        Li                   180.0      1_555  .      5_555  N
  Ta        O1        Li                   180.0      5_555  .      1_555  N
  Ta        O1        Li                     0.0      5_555  .      5_555  N
  Li        O1        Li                   180.0      1_555  .      5_555  N
  Sr        N1        Sr                   180.0      1_545  .      1_555  N
  Sr        N1        Sr                    90.0      1_545  .      2_555  N
  Sr        N1        Sr                    90.0      1_545  .      2_655  N
  Sr        N1        Ta                    90.0      1_545  .      1_555  N
  Sr        N1        Ta                    90.0      1_545  .      5_555  N
  Sr        N1        Li                    90.0      1_545  .      1_555  N
  Sr        N1        Li                    90.0      1_545  .      5_555  N
  Sr        N1        Sr                    90.0      1_555  .      2_555  N
  Sr        N1        Sr                    90.0      1_555  .      2_655  N
  Sr        N1        Ta                    90.0      1_555  .      1_555  N
  Sr        N1        Ta                    90.0      1_555  .      5_555  N
  Sr        N1        Li                    90.0      1_555  .      1_555  N
  Sr        N1        Li                    90.0      1_555  .      5_555  N
  Sr        N1        Sr                   180.0      2_555  .      2_655  N
  Sr        N1        Ta                    90.0      2_555  .      1_555  N
  Sr        N1        Ta                    90.0      2_555  .      5_555  N
  Sr        N1        Li                    90.0      2_555  .      1_555  N
  Sr        N1        Li                    90.0      2_555  .      5_555  N
  Sr        N1        Ta                    90.0      2_655  .      1_555  N
  Sr        N1        Ta                    90.0      2_655  .      5_555  N
  Sr        N1        Li                    90.0      2_655  .      1_555  N
  Sr        N1        Li                    90.0      2_655  .      5_555  N
  Ta        N1        Ta                   180.0      1_555  .      5_555  N
  Ta        N1        Li                     0.0      1_555  .      1_555  N
  Ta        N1        Li                   180.0      1_555  .      5_555  N
  Ta        N1        Li                   180.0      5_555  .      1_555  N
  Ta        N1        Li                     0.0      5_555  .      5_555  N
  Li        N1        Li                   180.0      1_555  .      5_555  N
  Sr        O2        Sr               89.628(5)      1_655  .      2_655  N
  Sr        O2        Sr                95.56(5)      1_655  .      5_654  N
  Sr        O2        Sr               174.81(5)      1_655  .      6_654  N
  Sr        O2        Ta              93.471(29)      1_655  .      1_655  N
  Sr        O2        Ta              93.471(29)      1_655  .    105_553  N
  Sr        O2        Li              93.471(29)      1_655  .      1_655  N
  Sr        O2        Li              93.471(29)      1_655  .    105_553  N
  Sr        O2        Sr               174.81(5)      2_655  .      5_654  N
  Sr        O2        Sr                85.18(4)      2_655  .      6_654  N
  Sr        O2        Ta              86.197(35)      2_655  .      1_655  N
  Sr        O2        Ta              86.197(35)      2_655  .    105_553  N
  Sr        O2        Li              86.197(35)      2_655  .      1_655  N
  Sr        O2        Li              86.197(35)      2_655  .    105_553  N
  Sr        O2        Sr               89.628(5)      5_654  .      6_654  N
  Sr        O2        Ta              93.471(29)      5_654  .      1_655  N
  Sr        O2        Ta              93.471(29)      5_654  .    105_553  N
  Sr        O2        Li              93.471(29)      5_654  .      1_655  N
  Sr        O2        Li              93.471(29)      5_654  .    105_553  N
  Sr        O2        Ta              86.197(35)      6_654  .      1_655  N
  Sr        O2        Ta              86.197(35)      6_654  .    105_553  N
  Sr        O2        Li              86.197(35)      6_654  .      1_655  N
  Sr        O2        Li              86.197(35)      6_654  .    105_553  N
  Ta        O2        Ta               169.66(9)      1_655  .    105_553  N
  Ta        O2        Li                     0.0      1_655  .      1_655  N
  Ta        O2        Li               169.66(9)      1_655  .    105_553  N
  Ta        O2        Li               169.66(9)    105_553  .      1_655  N
  Ta        O2        Li                     0.0    105_553  .    105_553  N
  Li        O2        Li               169.66(9)      1_655  .    105_553  N
  Sr        N2        Sr               89.628(5)      1_655  .      2_655  N
  Sr        N2        Sr                95.56(5)      1_655  .      5_654  N
  Sr        N2        Sr               174.81(5)      1_655  .      6_654  N
  Sr        N2        Ta              93.471(29)      1_655  .      1_655  N
  Sr        N2        Ta              93.471(29)      1_655  .    105_553  N
  Sr        N2        Li              93.471(29)      1_655  .      1_655  N
  Sr        N2        Li              93.471(29)      1_655  .    105_553  N
  Sr        N2        Sr               174.81(5)      2_655  .      5_654  N
  Sr        N2        Sr                85.18(4)      2_655  .      6_654  N
  Sr        N2        Ta              86.197(35)      2_655  .      1_655  N
  Sr        N2        Ta              86.197(35)      2_655  .    105_553  N
  Sr        N2        Li              86.197(35)      2_655  .      1_655  N
  Sr        N2        Li              86.197(35)      2_655  .    105_553  N
  Sr        N2        Sr               89.628(5)      5_654  .      6_654  N
  Sr        N2        Ta              93.471(29)      5_654  .      1_655  N
  Sr        N2        Ta              93.471(29)      5_654  .    105_553  N
  Sr        N2        Li              93.471(29)      5_654  .      1_655  N
  Sr        N2        Li              93.471(29)      5_654  .    105_553  N
  Sr        N2        Ta              86.197(35)      6_654  .      1_655  N
  Sr        N2        Ta              86.197(35)      6_654  .    105_553  N
  Sr        N2        Li              86.197(35)      6_654  .      1_655  N
  Sr        N2        Li              86.197(35)      6_654  .    105_553  N
  Ta        N2        Ta               169.66(9)      1_655  .    105_553  N
  Ta        N2        Li                     0.0      1_655  .      1_655  N
  Ta        N2        Li               169.66(9)      1_655  .    105_553  N
  Ta        N2        Li               169.66(9)    105_553  .      1_655  N
  Ta        N2        Li                     0.0    105_553  .    105_553  N
  Li        N2        Li               169.66(9)      1_655  .    105_553  N
#--eof--eof--eof--eof--eof--eof--eof--eof--eof--eof--eof--eof--eof--eof--eof--#
